Structures, Luminescence, and Magnetic Properties of Several Three-Dimensional Lanthanide‒Organic Frameworks Comprising 4-Carboxyphenoxy Acetic Acid
Shi, Peng-fei; Chen, Zhi; Xiong, Gang; Shen, Bo; Sun, Jing-Zhe; Cheng, Peng; Zhao, Bin; Crystal Growth & Design 12 (2012) 5203–; doi:10.1021/cg300277m

data_4506603
_publ_section_title
;
 Structures, Luminescence, and Magnetic Properties of Several
 Three-Dimensional Lanthanide--Organic Frameworks Comprising
 4-Carboxyphenoxy Acetic Acid
;
_journal_issue                   11
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              5203
_journal_paper_doi               10.1021/cg300277m
_journal_volume                  12
_journal_year                    2012
_chemical_formula_sum            'C10 H8 Dy O8'
_chemical_formula_weight         418.66
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   constr
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 96.025(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   7.3567(2)
_cell_length_b                   7.0497(2)
_cell_length_c                   23.4803(5)
_cell_measurement_temperature    293(2)
_cell_volume                     1211.02(5)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'SuperNova, Single source at offset), Eos'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0292
_diffrn_reflns_av_sigmaI/netI    0.0462
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_number            4273
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         2.78
_exptl_absorpt_coefficient_mu    6.203
_exptl_absorpt_correction_T_max  0.8860
_exptl_absorpt_correction_T_min  0.5759
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_density_diffrn    2.296
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             792
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.02
_refine_diff_density_max         2.730
_refine_diff_density_min         -2.093
_refine_diff_density_rms         0.265
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.026
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     166
_refine_ls_number_reflns         2135
_refine_ls_number_restraints     132
_refine_ls_restrained_S_all      0.996
_refine_ls_R_factor_all          0.0685
_refine_ls_R_factor_gt           0.0636
_refine_ls_shift/su_max          0.007
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0000P)^2^+160.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1603
_refine_ls_wR_factor_ref         0.1624
_reflns_number_gt                1984
_reflns_number_total             2135
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg300277m_si_002.cif
_cod_data_source_block           4a
_cod_original_sg_symbol_H-M      P21/c
_cod_database_code               4506603